Module III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina


 Kerrie Price
 1 years ago
 Views:
Transcription
1 Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the type of materials and tests conducted to find material constants are discussed first. Types of materials: The materials are classified based on the behaviour for a particular loading condition. These include, (i) Anisotropic materials (ii) Monoclinic materials (ii) Orthotropic materials (iii) Transversely isotropic materials (iv) Isotropic materials Anisotropic materials: In an anisotropic material, there are no planes of material property symmetry. So, it has different physical properties in different directions relative to the crystal orientation of the materials i.e., material properties are directionally dependent. σ 11 C 11 C 12 C 13 C 14 C 15 C 16 ε 11 σ 22 C 12 C 22 C 23 C 24 C 25 C 26 ε 22 σ 33 C 13 C 23 C 33 C 34 C 35 C 36 ε 33 ( 3.1) τ 23 = C 14 C 24 C 34 C 44 C 45 C 46 γ 23 τ 31 C 15 C 25 C 35 C 45 C 55 C 56 γ 31 τ 12 C 16 C 26 C 36 C 46 C 56 C 66 γ 12 Dept. of Aerospace Engg., Indian Institute of Technology, Madras 1
2 There are 21 independent elastic constants in the stressstrain relationship as given above. As shown in the above relations, there are couplings between the stresses and strains. Normal stresses produce not only normal strains in other directions due to Poisson effect but, also shear strains due to the effect of mutual influence. Similarly, shear stresses produce not only shear strains but also normal strains. In an anisotropic material, a combination of extensional and shear deformation is produced by a normal stress acting in any direction. This phenomenon of creating both extensional and shear deformations by the application of either normal or shear stresses is termed as extensionshear coupling and is not observed in isotropic materials. Monoclinic materials: It has a single plane of material property symmetry. If xy plane (i.e.; 12 plane) is considered as the plane of material symmetry then, there are 13 independent elastic constants in the stiffness matrix as given below. σ 11 C 11 C 12 C C 16 ε 11 σ 22 C 12 C 22 C C 26 ε 22 σ 33 τ 23 = C 13 C 23 C C C 44 C 45 0 ε 33 γ 23 ( 3.2) τ C 45 C 55 0 γ 31 τ 12 C 16 C 26 C C 66 γ 12 As there is a single plane of material property symmetry, shear stresses from the planes in which one of the axis is the perpendicular axis of the plane of material symmetry (i.e.; 23 and 31 planes) will contribute only to the shear strains in those planes. And normal stresses will not contribute any shear strains in these planes. Dept. of Aerospace Engg., Indian Institute of Technology, Madras 2
3 Orthotropic materials: There are three mutually orthogonal planes of material property symmetry in an orthotropic material. Fiberreinforced composites, in general, contain the three orthogonal planes of material property symmetry and are classified as orthotropic materials. The intersections of these three planes of symmetry are called the principal material directions. The material behaviour is called as specially orthotropic, when the normal stresses are applied in the principal material directions. Otherwise, it is called as general orthotropic which behaves almost equivalent to anisotropic material. There are nine independent elastic constants in the stiffness matrix as given below for a specially orthotropic material. σ 11 C 11 C 12 C ε 11 σ 22 C 12 C 22 C ε 22 σ 33 τ 23 = C 13 C 23 C C ε 33 γ 23 ( 3.3) τ C 55 0 γ 31 τ C 66 γ 12 From the stressstrain relationship it is clear that normal stresses applied in one of the principal material directions on an orthotropic material cause elongation in the direction of the applied stresses and contractions in the other two transverse directions. However, normal stresses applied in any directions other than the principal material directions create both extensional and shear deformations. Transversely isotropic materials: If a material has axes of symmetry in its longitudinal axis and all directions perpendicular to its longitudinal axis (i.e., more than three mutually perpendicular axes of symmetry) then such Dept. of Aerospace Engg., Indian Institute of Technology, Madras 3
4 material is transversely isotropic. (e.g., unidirectional composites). There are five independent elastic constants for these materials. σ 11 C 11 C 12 C ε 11 σ 22 C 12 C 11 C ε 22 σ 33 C 13 C 13 C ε 33 ( 3.4) τ 23 = C γ 23 τ C 44 0 γ 31 τ (C 11 C 12 ) γ 12 2 Isotropic material: In an isotropic material, properties are the same in all directions (axial, lateral, and in between). Thus, the material contains an infinite number of planes of material property symmetry passing through a point. i.e., material properties are directionally independent. So, there are two independent elastic constants. σ 11 C 11 C 12 C ε 11 σ 22 C 12 C 11 C ε 22 σ 33 = C 12 C 12 C ε 33 ( 3.5) τ (C 11 C 12 ) γ 23 τ (C 11 C 12 ) 0 2 γ 31 τ (C 11 C 12 ) 2 γ 12 Tensile normal stresses applied in any direction on an isotropic material cause only elongation in the direction of the applied stresses and contractions in the two transverse directions. It will not Dept. of Aerospace Engg., Indian Institute of Technology, Madras 4
5 produce any shear strain in any form in the material. Similarly, shear stresses produce only corresponding shear strains not normal strains. As the material properties are directionly independent, isotropic material has equal strength in all directions. As such, efficient structure (without wasting material structurally) is not possible by isotropic material (e.g., beam). In a beam the load is applied on the transverse direction and the beam will bend by extending and contracting in the lengthwise direction. In the lateral direction there is no load applied and the strength in the lateral direction is under utilized. Hence, isotropic material in beam structure is not efficient design, as the material is under utilized. On the other hand, unidirectional fibers which are aligned in the lengthwise direction will have high strength in the lengthwise direction and low strength in the other direction and thus, it becomes an efficient design. If the structure is taking complex loading system then, isotropic properties will be ideal and by arranging the fibers randomly quasi isotropic properties can be achieved. Isotropic Specially Orthotropic Anisotropic Figure 3.1 Differences in the deformations on uniaxial tension and pure shear From figure 3.1, it is clear that isotropic and specially orthotropic materials behave in a similar way. But, the magnitude of deformation is direction dependent in the case of orthotropic Dept. of Aerospace Engg., Indian Institute of Technology, Madras 5
6 whereas in the case of isotropic it is not. Anisotropic (and generally, orthotropic material) has coupling between normal and shear deformations. To summarize the elastic constants of each type of material is given in Table 1.27 Table 1.27: Elastic constants of different materials Three dimensional Two dimensional Material Number of Number of Number of Number of non zero independent non zero independent constants constants constants constants Anisotropic Generally Orthotropic Specially Orthotropic Transversely Isotropic Isotropic References : 1) Analysis and Performance of Fibre composites,  B.D. Agarwal, L.J. Broughtman and K.Chandrashekar John Wiley & Sons. Inc. 2) Principles of Composite Material Mechanics, R.F. Gibson, CRC Press. Dept. of Aerospace Engg., Indian Institute of Technology, Madras 6
7 Lecture 24 TwoDimensional Unidirectional Lamina: Consider, a thin plate of unidirectional composite material of uniform crosssection. If there are loads applied only along the edges and no outofplane loads, then, it can be considered to be a plane stress case. Figure 3.2 Orthotropic lamina Since, the plate is very thin, the stresses normal to plane of loading i.e. σ z, τ xz and τ yz can be assumed to vary insignificantly across the thickness. Thus, they can be assumed to be zero within the plate. i.e. σ z = 0, τ xz = 0, and τ yz = 0 ( 3.6) This assumption reduces the threedimensional stress strain equations to twodimensional stress strain equations. From generalized Hooke s law, If σ z = 0, then ( 3.7) ( 3.8) Let, the principal material directions be designated by the longitudinal direction L and the transverse direction T. Considering various loading conditions, the corresponding strains in the longitudinal and transverse directions are determined as follows. Dept. of Aerospace Engg., Indian Institute of Technology, Madras 7
8 Case (i) Only longitudinal load is applied Therefore,, ( 3.9) Figure 3.3 Longitudinal loading condition The strains corresponding to this loading condition are, ( 3.10) ( 3.11) ( 3.12) Case (ii) Only transverse load is applied Therefore,, Figure 3.4 Transverse loading condition The strains corresponding to this loading condition are, ( 3.13) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 8
9 ( 3.14) Case (iii) Only shear load is applied Therefore,, τ LT Figure 3.5 Shear loading condition The strains corresponding to this loading condition are, ( 3.15) Case (iv) All loads are applied Superimposing cases (i), (ii) and (iii) ( 3.16) σ T τ LT σ L σ L τ LT σ T Figure 3.6 Lamina under loading condition Dept. of Aerospace Engg., Indian Institute of Technology, Madras 9
10 The strains corresponding to this loading condition are, ( 3.17) ( 3.18) Anisotropic layer (Generally Orthotropic): When an orthotropic lamina is loaded in the direction other than its principal material axes, then, the behaviour of the lamina will be anisotropic. In the figure 3.7, the lamina will behave like anisotropic if load is applied along x or y directions. θ Figure 3.7 Generally Orthotropic lamina Case (i) Only longitudinal load is applied (along x direction) Therefore, σ x σ x Figure 3.8 Longitudinal loading condition The strains corresponding to this loading condition are, ( 3.19) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 10
11 ( 3.20) where, m x is the coefficient of mutual influence and E L is the modulus of composite along L direction ( 3.21) Case (ii) Only transverse load is applied Therefore, σ y σ y Figure 3.9 Transverse loading condition The strains corresponding to this loading condition are, ( 3.22) ( 3.23) ( 3.24) Case (ii) Only shear load is applied Therefore, Dept. of Aerospace Engg., Indian Institute of Technology, Madras 11
12 τ xy τ xy Figure 3.10 Shear loading condition The strains corresponding to this loading condition are, ( 3.25) ( 3.26) ( 3.27) Case (iv) All loads are applied Superimposing cases (i), (ii) and (iii) ( 3.28) ( 3.29) ( 3.30) References : 1) Analysis and Performance of Fibre composites,  B.D. Agarwal, L.J. Broughtman and K.Chandrashekar John Wiley & Sons. Inc. 2) Principles of Composite Material Mechanics, R.F. Gibson, CRC Press. Dept. of Aerospace Engg., Indian Institute of Technology, Madras 12
13 Problems : Calculate E x, E y, γ xy, M x and G LT = 4 GPa and γ CT = 0.4. M y at 45 o draw orthotropic lamina of E L = 35 GPa, E T = 3.5 GPa, Find, x, y, xy when, σ = 20 MPa. x Lecture 25 Transformation of Engineering constants: It is of interest to derive and know the explicit expressions for the usual engineering constants in the arbitrary axes in terms of those, along the principal material axes. Consider an orthotropic lamina with its principal material axes (L and T) oriented at an angle θ with reference axes (x and y) as shown in Fig θ Fig Orthotropic lamina Let, the only nonzero stress acting on this lamina be σ x. i.e., The normal and shearing stresses along the L and T directions can be calculated by the stresstransformation law: σ σ θ σ θ τ θ θ 2 L = x cos + y sin Xy sin cos = ( 3.31) 2 σl σxcos θ σ σ θ σ θ τ θ θ 2 T = x sin + y cos 2 2 Xy sin cos Dept. of Aerospace Engg., Indian Institute of Technology, Madras 13
14 = ( 3.32) 2 σt σxsin θ ( ) τ = σ sinθ cosθ + σ sinθ cosθ + τ cos 2θ sin 2θ LT x y xy τ = σ sinθcosθ ( 3.33) LT x The above relations are substituted in the strain relations derived previously for the orthotropic lamina in the L and T directions. ( 3.34) ( 3.35) ( 3.36) The strains in the x and y directions can be obtained as by taking the inverse of the straintransformation law, which can be written as : ( 3.37) ( 3.38) ( 3.39) Substitution of the values of ε L, ε T, and γ LT the above equations become, Dept. of Aerospace Engg., Indian Institute of Technology, Madras 14
15 ( 3.40) ( 3.41) From trigonometry: ( 3.42) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 15
16 ( 3.43) ( 3.44) ( 3.45) To summarize, ( 3.46) ( 3.47) ( 3.47) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 16
17 Determinations of Elastic constants Once the strains are found, the elastic constants can be determined from the Hooke's law. The modulus of elasticity in the xdirection is given by : From the previous equation for ε x, E x can be calculated as : ( 3.48) ( 3.49) The expression for E y can be obtained by substituting θ + 90º for θ in above equation : ( 3.50) The Poisson ratio is defined as : ( 3.51) ( 3.52) Similarly, ( 3.53) ( 3.54) When the normal stress σ x is applied in a direction other than the L and T direction, it may induce a shearing strain given by the above equations. Therefore, a coefficient of mutual influence, m x, may be defined that relates the shearing strain to the normal stress σ x in the following manner: ( 3.55) ( 3.56) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 17
18 Substituting the values σ x and γ xy, Similarly, the coefficient, m y, which relates the shearing strain to normal stress σ y is defined as : ( 3.57) ( 3.58) To obtain an expression for G xy, assume that the only nonzero stress acting on the lamina is τ xy (Pure shear case). The stresses along the principal material directions are given by : ( 3.59) ( 3.60) ( 3.61) ( 3.62) The corresponding strains are given by Hooke s law, ( 3.63) ( 3.64) ( 3.65) Substitution of the above equations gives the shearing strain γ xy, Dept. of Aerospace Engg., Indian Institute of Technology, Madras 18
19 ( 3.66) ( 3.67) As the normal stresses do, the shearing stress τ xy will also cause direct strains ε x, and ε y in the x and y directions, respectively, given by : ( 3.68) ( 3.69) It will be relevant at this point to note that the stressstrain relations for an orthotropic lamina referred to arbitrary axes can be written in terms of engineering constants as : ( 3.70) ( 3.71) ( 3.72) The elastic constants E x, E y, ν xy, ν yx, m x, m y, and G xy are determined from the equations given above. Dept. of Aerospace Engg., Indian Institute of Technology, Madras 19
20 Lecture 26 Specially Orthotropic material under Plane stress: In plane stress condition, the stresses normal to the plane under consideration are assumed to be zero. i.e., if the 12 (xy) plane is assumed to be the loading plane, then the normal stresses to 12 plane σ3 = τ23 = τ13 = 0 ( 3.73) Fig Orthotropic lamina More over, the number of independent elastic constants for orthotropic material in the plane stress condition are reduced to 4 from 9 in the threedimensional case. Thus, the stressstrain relation is given by σ 11 C 11 C 12 C ε 11 σ 22 C 12 C 22 C ε 22 σ 33 = 0 τ 23 = 0 = C 13 C 23 C C ε 33 γ 23 ( 3.74) τ 31 = C 55 0 γ 31 τ C 66 γ 12 σ 11 = C 11 ε 11 + C 12 ε 22 + C 13 ε 33 ( 3.75) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 20
21 σ 22 = C 12 ε 11 + C 22 ε 22 + C 23 ε 33 ( 3.76) 0 = C 13 ε 11 + C 32 ε 22 + C 33 ε 33 γ 23 = 0 γ 13 = 0 τ 12 = C 66 γ 12 after eliminating ε 33, the equations may be written as σ C1 32 C13C23 11 or σ 1 = c11 1 c12 2 C ε + 33 C ε 33 σ c13 c23 C2 22 or σ 2 c c22 2 c ε = + 33 C ε 33 ( 3.77) ( 3.78) or, τ 12 = C 66 γ 12 ( 3.79) σ1 Q11 Q12 0 ε1 σ2 = Q12 Q22 0 ε2 τ Q γ ( 3.80) where, Q C = c C Q C = c C ( 3.81) ( 3.82) Q = c C C C ( 3.83) for specially orthotropic composite materials, the stiffness coefficients may be related with engineering constants as follows: Dept. of Aerospace Engg., Indian Institute of Technology, Madras 21
22 Q 12 Q Q = EL 1 ν ν ( 3.84) LT TL = ET 1 ν ν ( 3.85) LT TL νlt ET νtl EL = = 1 ν ν 1 ν ν LT TL LT TL ( 3.86) Q 66 = GLT ( 3.87) The strainstress relationship is given by, where ( 3.88) ( 3.89) ( 3.90) ( 3.91) ( 3.92) Stressstrain relations for thin isotropic lamina: Stresses in an isotropic lamina under a plane stress condition is given by ( 3.93) where ( 3.94) ( 3.95) and the strainstress relation is given by ( 3.96) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 22
23 where, ( 3.97) ( 3.98) ( 3.99) ( 3.100) Lecture 27 Stressstrain relations for lamina with arbitrary orientation: Consider an orthotropic lamina with its principal material axes oriented at an angle θ with the reference coordinate axes as shown in figure. Stresses and strains can be easily transformed from one set of axes to another. Fig lamina with arbitrary orientation From elementary mechanics of materials the transformation equations for expressing stresses in a 12 coordinate system in terms of stresses in a xy coordinate system, Dept. of Aerospace Engg., Indian Institute of Technology, Madras 23
24 ( 3.101) The transformations are commonly written as ( 3.102) ( 3.103) ( 3.104) where, the transformation matrix is given by ( 3.105) ( 3.106) where, [R] is the Reuter matrix and is defined as ( 3.107) ( 3.108) For a specially orthotropic lamina whose principal material axes are aligned with the natural body axes, ( 3.109) ( 3.110) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 24
25 (3.111) ( 3.112) ( 3.113) However, = ( 3.114) ( 3.115) where, is the transformed reduced stiffness matrix. ( 3.116) [ ( 3.117) Thus, the stressstrain relations in xy coordinates are where, ( ) Q11 = Q11 cos θ + Q22 sin θ + 2 Q12 + 2Q66 sin θcos θ ( ) Q22 = Q11 sin θ + Q22 cos θ + 2 Q12 + 2Q66 sin θcos θ ( 4 ) sin 2 θcos 2 θ ( sin 4 θ cos 4 θ) Q = Q + Q Q + Q ( ) ( ) Q = Q Q 2Q sinθcos θ Q Q 2Q sin θcosθ ( ) ( ) Q = Q Q 2Q sin θcosθ Q Q 2Q sinθcos θ ( 2 2 ) sin 2 θcos 2 θ ( sin 4 θ cos 4 θ) Q = Q + Q Q Q + Q ( 3.118) ( 3.119) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 25
26 If θ = 0 o, If θ = 90 o, ( 3.120) ( 3.121) Similarly, the strainstress relation along the principal axes for a specially orthotropic lamina can be written as : Therefore, the strainstress relation along any arbitrary direction is given by ( 3.122) where, Ŝ is the transformed reduced compliance matrix Ŝ = [T] T [S][T] and ( 3.123) Thus, the strainstress relations in xy coordinates are ( 3.124) ( 3.125) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 26
27 where, ( ) S = S cos θ + S sin θ + 2 S + 2S sin θcos θ ( ) S = S sin θ + S cos θ + 2 S + 2 S sin θcos θ ( ) sin 2 θcos 2 θ ( sin 4 θ cos 4 θ) S = S + S S + S ( ) ( ) S = 2S 2S S sinθcos θ 2S 2 S S sin θcosθ ( ) ( ) S = 2S 2S SQ sin θcosθ 2S 2S S sinθcos θ ( ) θ θ ( θ θ) S = 2 2S + 2 S 4 S S sin cos S sin + cos (3.126) If θ = 0 o, ; ; ; ; If θ = 90 o, ( 3.127) ; ; ; ; ( 3.128) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 27
28 Lecture 28 Mechanical properties of Composites: The mechanical properties of composite materials are determined by conducting standard tests framed by the American Society for Testing and Materials (ASTM). The followings are the list of ASTM standards, which are used to find the mechanical properties of composite materials. Tensile test  ASTM D3039 Compression test  ASTM D3410 Flexural test  ASTM D790 ±45 Shear test  ASTM D3518 Inplane Shear test  ASTM D4255 Interlaminar shear strength  ASTM D2344 Tensile Strength test: The tensile properties of composite laminate are determined in accordance with ASTM D3039. The tensile specimen is straightsided and has the crosssection as shown in the figure. Specimen thickness End tab 38 mm Gauge length + 2* width 38 mm Figure 3.14 tensile test specimen The tensile specimen is held in the testing machine by wedge action grips. Longitudinal and transverse strains are measured using strain gauges. Longitudinal tensile modulus E 11 and the major Poisson's ratio ν 12 are determined from the tension test data of 0 o unidirectional laminates. The transverse modulus E 22 and the minor Poisson's ratio ν 21 are determined from the tension test data of 90 o unidirectional laminates. Dept. of Aerospace Engg., Indian Institute of Technology, Madras 28
29 Figure 3.15 Tensile test apparatus For an offaxis unidirectional specimen (0 o < θ < 90 o ), a tensile load creates both extension and shear deformations (since A 16 and A 26 are not equal to zero). Hence, the experimentally determined modulus of an offaxis specimen is corrected to obtain its true modulus using the equation: E true = (1η) E experimental ( 3.129) where, η = 3*S 2 16 / (S 2 11 [3*(S 66 /S 11 ) + 2*(L/w) 2 ]) ( 3.130) L  the specimen length between grips w  the specimen width S ij  the elements in the compliance matrix Flexural Strength test: Flexural strength and modulus are determined by ASTM test method D790. In this test, a rectangular cross section of composite beam speciment is loaded in a threepoint bending mode. P d b L/2 L/2 Figure 3.16 Flexural test setup Dept. of Aerospace Engg., Indian Institute of Technology, Madras 29
30 Figure 3.17 Flexural test apparatus  Three point loading The maximum fiber stress at failure on the tension side of a flexural specimen is considered the flexural strength of the material. Therefore, the flexural strength is given by : ( 3.131) ( 3.132) 3Pl σ = 2 ( 3.133) 2bd Interlaminar Shear Strength (ILSS): Interlaminar shear strength of composite is the shear strength parallel to the plane of laminate. It is determined in accordance with ASTM D2344 using a shortbeam shear test. It is applicable to all types of parallel fiber reinforced plastics and composites. The thickness and width of the test specimen are measured before conditioning. The specimen is placed on a horizontal shear test fixture so that the fibers are parallel to the loading nose. The loading nose is then used to flex the specimen at a speed of.05 inches per minute until Dept. of Aerospace Engg., Indian Institute of Technology, Madras 30
31 breakage. The force is then recorded. To determine shear strength, calculations are performed as given below. P L/2 L/2 b d Figure 3.18 Short beam shear test ( 3.134) ( 3.135) ( 3.136) InPlane Shear Strength (IPSS): ( 3.137) The shear modulus G 12 and the ultimate shear strength τ 12U of unidirectional fiberreinforced composites may be determined by any one of the following test procedures. (i) ± 45 o shear test (ASTM D3518) (ii) Iosipescu or Vnotched shear test (ASTM D5379) (iii) Tworail or threerail shear test (ASTM D4255) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 31
32 25.4 mm End tab 38.5 mm 178 mm End tab 38.5 mm P Figure 3.19 ± 45 o shear test configuration In ± 45 o shear test, test specimens are placed in the grips of a universal tester at a specified grip separation and pulled until failure. Optional tabs can be bonded to the ends of the specimen to prevent gripping damage. The expressions to find the shear modulus and the shear strength is given by the expressions σ xx G 12 = 2 ( εxx εyy ) ( 3.138) The shear strength is given by the expression S P 2bh max 12 = ( 3.139) Dept. of Aerospace Engg., Indian Institute of Technology, Madras 32
33 Figure 3.20 Vnotched shear test The Iosipescu or Vnotched shear test uses a rectangular beam with symmetrical centrally located Vnotches. The beam is loaded by a special fixture applying a shear loading at the V notch. Either inplane or outofplane shear properties may be evaluated, depending upon the orientation of the material coordinate system relative to the loading axis. The notched specimen is loaded by introducing a relative displacement between two halves of the test fixture. The shear stress is calculated as where P τ = ( 3.140) wh P  applied load w  distance between the notches h  specimen thickness Dept. of Aerospace Engg., Indian Institute of Technology, Madras 33
34 Figure 3.21 Tworail shear test In tworail shear test, two pairs of steel rails are fastened along the long edges of a 76.2 mm wide and mm long rectangular specimen, usually by three bolts on each side. At the other two edges, the specimen remains free. A tensile load is applied to the rails. That will induce an inplane shear load on the tested laminate. The shear strength is calculated by using the expression P τ = ( 3.141) Lh where, L  the specimen length h  the specimen thickness Dept. of Aerospace Engg., Indian Institute of Technology, Madras 34
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationME 243. Mechanics of Solids
ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET Email: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil
More informationINTRODUCTION TO STRAIN
SIMPLE STRAIN INTRODUCTION TO STRAIN In general terms, Strain is a geometric quantity that measures the deformation of a body. There are two types of strain: normal strain: characterizes dimensional changes,
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationModule 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations
Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates CrossPly Laminates Specially Orthotropic Laminates Examples Homework References
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationLab Exercise #5: Tension and Bending with Strain Gages
Lab Exercise #5: Tension and Bending with Strain Gages Prelab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationAmerican Society for Testing and Materials (ASTM) Standards. Mechanical Testing of Composites and their Constituents
Mechanical Testing of Composites and their Constituents American Society for Testing and Materials (ASTM) Standards Tests done to determine intrinsic material properties such as modulus and strength for
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationChapter 5 PlaneStress StressStrain Relations in a Global Coordinate System
Chapter 5 PlaneStress StressStrain Relations in a Global Coordinate System One of the most important characteristics of structures made of fiberreinforced materials, and one which dictates the manner
More informationConstitutive Equations
Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationMechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces
Mechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces PingCheung Tse epartment of Mechanical Engineering, The Hong Kong Polytechnic University, Hunghom, Kowloon, Hong Kong
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More information8 Properties of Lamina
8 Properties of Lamina 8 ORTHOTROPIC LAMINA An orthotropic lamina is a sheet with unique and predictable properties and consists of an assemblage of fibers ling in the plane of the sheet and held in place
More informationStress, Strain, Mohr s Circle
Stress, Strain, Mohr s Circle The fundamental quantities in solid mechanics are stresses and strains. In accordance with the continuum mechanics assumption, the molecular structure of materials is neglected
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More informationELASTICITY (MDM 10203)
ELASTICITY () Lecture Module 3: Fundamental Stress and Strain University Tun Hussein Onn Malaysia Normal Stress inconstant stress distribution σ= dp da P = da A dimensional Area of σ and A σ A 3 dimensional
More informationMechanical Behavior of Composite Tapered Lamina
International Journal of Engineering Research and Development eissn: 2278067X, pissn: 2278800X, www.ijerd.com Volume 10, Issue 8 (August 2014), PP.1927 Mechanical Behavior of Composite Tapered Lamina
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationSTANDARD SAMPLE. Reduced section " Diameter. Diameter. 2" Gauge length. Radius
MATERIAL PROPERTIES TENSILE MEASUREMENT F l l 0 A 0 F STANDARD SAMPLE Reduced section 2 " 1 4 0.505" Diameter 3 4 " Diameter 2" Gauge length 3 8 " Radius TYPICAL APPARATUS Load cell Extensometer Specimen
More informationSEMM Mechanics PhD Preliminary Exam Spring Consider a twodimensional rigid motion, whose displacement field is given by
SEMM Mechanics PhD Preliminary Exam Spring 2014 1. Consider a twodimensional rigid motion, whose displacement field is given by u(x) = [cos(β)x 1 + sin(β)x 2 X 1 ]e 1 + [ sin(β)x 1 + cos(β)x 2 X 2 ]e
More informationLearning Units of Module 3
Module Learning Units of Module M. tresstrain oncepts in Three Dimension M. Introduction to Anisotropic lasticity M. Tensorial oncept and Indicial Notations M.4 Plane tress oncept Action of force (F)
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationDAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES
DAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES M. Kawai Institute of Engineering Mechanics University of Tsukuba,
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 34 Thermal Stresses in Plates Lecture Overview Introduction Mechanical and Thermal Strains
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationBasic Equations of Elasticity
A Basic Equations of Elasticity A.1 STRESS The state of stress at any point in a loaded bo is defined completely in terms of the nine components of stress: σ xx,σ yy,σ zz,σ xy,σ yx,σ yz,σ zy,σ zx,andσ
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationDYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD
ECCM66 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 6 June 4 DYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD K. V. Nagendra Gopal a*,
More information[8] Bending and Shear Loading of Beams
[8] Bending and Shear Loading of Beams Page 1 of 28 [8] Bending and Shear Loading of Beams [8.1] Bending of Beams (will not be covered in class) [8.2] Bending Strain and Stress [8.3] Shear in Straight
More informationProject MMS13 Task 5 Report No 3 (M6/D3)
Project MMS13 Task 5 Report No 3 (M6/D3) Material Data Requirements and Recommended Test Methods for the Predictive Modelling of Defect Criticality in Composite Material Systems M R L Gower and G D Sims
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationModule 2 Stresses in machine elements. Version 2 ME, IIT Kharagpur
Module Stresses in machine elements Lesson Compound stresses in machine parts Instructional Objectives t the end of this lesson, the student should be able to understand Elements of force system at a beam
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationEvaluation of inplane orthotropic elastic constants of paper and paperboard
Evaluation of inplane orthotropic elastic constants of paper and paperboard T. Yokoyama and K. Nakai Department of Mechanical Engineering, Okayama University of Science  Ridaicho, Okayama 75, Japan
More informationChapter 2: Elasticity
OHP 1 Mechanical Properties of Materials Chapter 2: lasticity Prof. Wenjea J. Tseng ( 曾文甲 ) Department of Materials ngineering National Chung Hsing University wenjea@dragon.nchu.edu.tw Reference: W.F.
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationLecture 15 Strain and stress in beams
Spring, 2019 ME 323 Mechanics of Materials Lecture 15 Strain and stress in beams Reading assignment: 6.1 6.2 News: Instructor: Prof. Marcial Gonzalez Last modified: 1/6/19 9:42:38 PM Beam theory (@ ME
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationPurpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on Exam 3.
ES230 STRENGTH OF MTERILS Exam 3 Study Guide Exam 3: Wednesday, March 8 th inclass Updated 3/3/17 Purpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationMechanical behaviour of wood in the orthotropic directions
Mechanical behaviour of wood in the orthotropic directions J.. Morais 1, J. C. Xavier 1, N. M. Dourado 1, J.. ousada 2 1 Departamento de Engenharias, ICETA/UTAD, Portugal 2 Departamento de Florestal, ICETA/UTAD,
More informationVYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA
VYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA FAKULTA METALURGIE A MATERIÁLOVÉHO INŽENÝRSTVÍ APPLIED MECHANICS Study Support Leo Václavek Ostrava 2015 Title:Applied Mechanics Code: Author: doc. Ing.
More informationVIBRATION CONTROL OF RECTANGULAR CROSSPLY FRP PLATES USING PZT MATERIALS
Journal of Engineering Science and Technology Vol. 12, No. 12 (217) 33983411 School of Engineering, Taylor s University VIBRATION CONTROL OF RECTANGULAR CROSSPLY FRP PLATES USING PZT MATERIALS DILEEP
More informationBending Load & Calibration Module
Bending Load & Calibration Module Objectives After completing this module, students shall be able to: 1) Conduct laboratory work to validate beam bending stress equations. 2) Develop an understanding of
More informationTRESS  STRAIN RELATIONS
TRESS  STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown.
D : SOLID MECHANICS Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown. Q.2 Consider the forces of magnitude F acting on the sides of the regular hexagon having
More informationMechanics of Earthquakes and Faulting
Mechanics of Earthquakes and Faulting www.geosc.psu.edu/courses/geosc508 Surface and body forces Tensors, Mohr circles. Theoretical strength of materials Defects Stress concentrations Griffith failure
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationStress intensity factors for an inclined and/or eccentric crack in a finite orthotropic lamina
1886 Stress intensity factors for an inclined and/or eccentric crack in a finite orthotropic lamina Abstract Stress intensity factors (SIF) are determined for an inclined and / or eccentric crack in a
More informationGEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE
GEOSYNTHETICS ENGINEERING: IN THEORY AND PRACTICE Prof. J. N. Mandal Department of Civil Engineering, IIT Bombay, Powai, Mumbai 400076, India. Tel.02225767328 email: cejnm@civil.iitb.ac.in Module13 LECTURE
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationRELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer
RELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer and Robert J. Ross Supervisory Research Engineer USDA Forest Service Forest Products
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More information